* Your assessment is very important for improving the work of artificial intelligence, which forms the content of this project
Journal of Macromolecular Science, Part C: Polymer Reviews ISSN: 1532-1797 (Print) 1520-5746 (Online) Journal homepage: http://www.tandfonline.com/loi/lmsc19 Synthesis of Poly(Lactic Acid): A Review Rajeev Mehta , Vineet Kumar , Haripada Bhunia & S. N. Upadhyay To cite this article: Rajeev Mehta , Vineet Kumar , Haripada Bhunia & S. N. Upadhyay (2005) Synthesis of Poly(Lactic Acid): A Review, Journal of Macromolecular Science, Part C: Polymer Reviews, 45:4, 325-349, DOI: 10.1080/15321790500304148 To link to this article: https://doi.org/10.1080/15321790500304148 Published online: 21 Aug 2006. Submit your article to this journal Article views: 3381 Citing articles: 176 View citing articles Full Terms & Conditions of access and use can be found at http://www.tandfonline.com/action/journalInformation?journalCode=lmsc19 Journal of Macromolecular Sciencew, Part C: Polymer Reviews, 45:325–349, 2005 Copyright # Taylor & Francis, Inc. ISSN 1532-1797 print/1532-9038 online DOI: 10.1080/15321790500304148 Synthesis of Poly(Lactic Acid): A Review RAJEEV MEHTA,1 VINEET KUMAR,1 HARIPADA BHUNIA,1 AND S. N. UPADHYAY2 1 Department of Chemical Engineering, Thapar Institute of Engineering and Technology, Patiala, Punjab, India 2 Department of Chemical Engineering and Technology, Institute of Technology, Banaras Hindu University, Varanasi, India Poly(lactic acid), a bio-degradable polymer, has been studied extensively during the past 15 years. This paper presents a review on poly(lactic acid) (PLA) with focus on its stereochemistry, synthesis via ring-opening polymerization, reaction kinetics and thermodynamics, synthesis of low molecular weight polymer, a continuous process for production of PLA from lactic acid, and blends. The different polymerization mechanisms, which have been proposed in the literature, are also summarized. Various catalyst systems, solvents, and reaction temperature and time give products of an entire range of molecular weights, ranging from a few thousand to over a million. Modeling and simulation of the ring-opening polymerization of PLA is also discussed. Keywords poly(lactic acid), bio-degradable polymer, ring-opening polymerization, dehydratization, blends, modeling and simulation Introduction Worldwide production of high-volume consumer plastics continues to be dominated by petroleum-based polymers. Two factors have made biodegradable polymers economically attractive. These are (i) environmental and economic concerns associated with waste disposal and (ii) rising costs of petroleum production resulting form the depletion of the most easily accessible reserves. Ease of degradability, versatility and anticipated price as well as performance of the new generation of polymer, polylactic acid (PLA), will enable it to displace a significant volume of fossil fuel-based polymers. Poly(glycolic acid) (PGA) was the first biodegradable polymer synthesized (1). It was followed by poly(lactic acid) (PLA) and copolymers of the two (2). These a-polyesters have been investigated for use as sutures and as implant materials for repairing a variety of tissues (3). ‘Vicryl’ suture, a blend of PGA (90%) and PLA (10%) was introduced in USA in 1974. PLA was discovered in 1932 by Carothers (DuPont) who produced a low Received 20 May 2005, Accepted 1 August 2005 Address correspondence to S. N. Upadhyay, Department of Chemical Engineering and Technology, Institute of Technology, Banaras Hindu University, Varanasi, India 221005. Tel.: þ91-542-2317179; Fax: þ91-542-2368428; E-mail: [email protected] 325 326 R. Mehta et al. molecular weight product by heating lactic acid under vacuum. The inability, at that time to increase the molecular weight of the product, led to discontinuation of further studies. Later on, high molecular weight PLA was synthesized by ring-opening polymerization of lactide. According to the European Society for Biomaterials (4) ‘biodegradation’ is a process in which biological agents (enzymes or microbes) play a dominant role in the degradation process. Unlike other biodegradable polymers the degradation of PLA is not biodegradation as it is caused by hydrolytic cleavage of the polymer backbone, with little or no evidence of participation of enzymes. However, PLA is commonly termed as a biodegradable polymer. PLA can be manufactured with a wide range of properties, because of lactic acid being chiral with two asymmetric centers existing in four different forms. It can be made into a polymer with molecular weight ranging from a few thousands to over a million. It can be easily converted into film, fiber, spun bond, and melt blown products on existing processing equipment. PLA has practical medical applications as dissolvable sutures, as matrices for drug delivery, and bone fracture internal fixation devices in surgery (5). Other applications include its role as agricultural plant growth promoter, in textiles, and non-woven applications such as fiberfill, crop covers, geotextiles, wipes, diapers, binder fibers, etc. However, the total volume of PLA production remains small compared to other polymers (for e.g. PE reached a global level of 54 million tones in 2001, which can be compared to the figure of about 390,000 tonnes for PLA which is expected to be produced by 2008). The major driver for PLA production is its high volume use as fibers. PLA was developed as an alternative binder for cellulosic non-wovens because of its ease of hydrolysis compared with polyvinyl acetate or ethylene-acrylic acid copolymers. Spunlaid and melt-blown non-wovens based on PLA were researched at the University of Tennessee, Knoxville in 1993 (6). Kanebo (Japan) introduced Lactronw (poly L -lactide) fiber and spun-laid non-wovens in 1994 claiming a capacity of 2000 tons per annum, later expanded to 3000 tons per annum. It targeted agricultural applications to start with, and in 1998 was re-launched for apparel end-uses. At that time, Japanese demand for PLA fibers was said to be 500 –1000 tons per annum. In order to improve the biodegradability and reduce the cost of the non-wovens, blends with rayon were also developed. Cargil Dow Polymers LLC, the present leader in polylactic acid technology, is a 50-50 joint-venture between Cargill and Dow and was formed in November 1997. In 2004, they started the world’s first full-scale PLA plant in Blair, Nebraska, capable of producing 140,000 tons per annum. Polylactic acid, first synthesized about 50 years ago, has finally arrived as an alternative to PET, HIPS, PVC, and cellulosics in some high-clarity packaging roles. PLA is being used in candy wrap, optically enhanced films, and shrink labels. It is also showing up as the sealant layer in form-fill-seal coextrusions. The novel resin is forging roles in thermoformed cups and containers and is about to appear in single-serve drink bottles. A comparison of the mechanical and barrier properties of PLA and some other polymers is given in Tables 1 and 2 , and 3 (7, 8). Recent developments in the capability to manufacture the monomer economically from renewable feed stocks have placed these materials at the forefront of the emerging biodegradable plastics industry. Increasing realization of the intrinsic properties of these polymers, coupled with the knowledge of how such properties can be manipulated to achieve compatibility with thermoplastics processing, manufacturing, and end-use requirements, have fuelled the technological and commercial interests in PLA products. Synthesis of Poly(Lactic Acid) 327 Table 1 Properties of biaxially oriented films (7) Density, g/cc Haze, % Tensile str., psi, MD, Tensile mod., psi, MD Ult. elongation, %, MD Tear, g/mil, MD a PLA PP PET Nylon Cellophane 1.25 2.1 15,950 478,500 160 15 0.9 1– 4 27,550a 348,000 110a 4– 6 1.4 2 –5 29,725a 551,000a 140a 18 1.2 2– 3 36,250 264,625 125a 13 1.45 1 –2 13,050a 594,500a 23a 4 Median of a range of values. The objective of this review is to present a comprehensive picture of PLA synthesis, with emphasis on the various catalysts and some of the polymerization mechanisms, used for ring-opening polymerization. Monomer An important feature of lactic acid is that it exists in two optically active forms (Fig. 1). Fermentation derived lactic acid consists of 99.5% of the L -isomer. Production of the cyclic lactide dimer intermediate results in three potential forms. The D - and L -forms are optically active, the D,L - or meso-form is optically inactive. The ratio of these three forms is readily controlled in the process. Ring opening polymerization of the lactide results in a “family” of polymers containing different isomer ratios and in a range of molecular weights. Polymers with high L -levels can be used to produce crystalline products whereas the higher D -levels (.15%) result in an amorphous product. The thermal, mechanical, and biodegradation characteristics of lactic acid polymers are known to depend on the choice and distribution of stereoisomers within the polymer chains. High-purity L - and D -lactides form stereo regular isotactic poly(L -lactide) Table 2 Barrier performance of clear resins (7) Permeationb Polymer MVTRa Oxygen CO2 PLA HIPS Nylon 6 PET PP PVC 21 10 23 1 0.7 2 40 300– 400 3 3– 6 150 5– 20 183 NA NA 15 –25 NA 20 –50 a g-mil/100 in. 2-day. cc-mil/100 in. 2-day-atm. b 328 R. Mehta et al. Table 3 Mechanical properties of PGA and PLAa Elongation Polymer PGA (MW: 50,000) PLA L -PLA (MW:50,000) L -PLA (MW: 1,00,000) L -PLA (MW: 3,00,000) D ,L -PLA (MW:20,000) D ,L -PLA (MW:1,07,000) D ,L -PLA (MW: 5,50,000) Glass transition (8C) Melting temp. (8C) Tensile strength (MPa) Flexural modulus (MPa) Yield (%) Break (%) 35 210 n/a n/a n/a n/a 54 170 28 1400 3.7 6.0 58 159 50 3000 2.6 3.3 59 178 48 3250 1.8 2.0 50 — n/a n/a n/a n/a 51 — 29 1950 4.0 6.0 53 — 35 2350 3.5 5.0 a Based on data published by Engleberg and Kohn (8). n/a ¼ not available. (—) ¼ not applicable. (PLLA) and poly(D -lactide) (PDLA), respectively. These are semi crystalline polymers with a high melting point 1808C and a glass transition temperature in the 55 –608C range. The degree of crystallinity depends on many factors, such as molecular weight, thermal and processing history, and the temperature and time of annealing treatments. The meso- and D,L -lactide, on the other hand, form atactic poly (D,L -lactide) (PDLLA) which is amorphous (9). The mechanical properties and degradation kinetics of the semi-crystalline PLLA are quite different from those of completely amorphous PDLLA. Figure 1. Three different lactides. Synthesis of Poly(Lactic Acid) 329 Figure 2. PLA lifecycle. In particular, PLLA is always preferred whenever higher mechanical strength and longer degradation time is required (10). The PLA lifecycle is shown in Fig. 2. After formation of PLA oligomers from lactic acid by removal of water, depolymerization of oligomers takes place to give a thermodynamically favored lactide. This monomer is readily polymerized under vacuum distillation. It is used to produce high molecular weight PLA by ring-opening polymerization. The high molecular weight PLA can be degraded to lactic acid in presence of water. Synthesis of Polylactic Acid from Lactic Acid Synthesis of Low Molecular Weight Polylactic Acid by Condensation Polymerization There are two major routes to produce polylactic acid from the lactic acid monomer (Fig. 3). Route 1 involves removal of water of condensation by the use of solvent under high vacuum and high temperature. Polycondensation of lactic acid is usually performed in bulk by distillation of condensation water, with or without a catalyst, while vacuum and temperature are progressively increased. Although, high molecular weight polyesters with good mechanical properties are not easy to obtain, the properties of lactic acid oligomers, which can be further used as intermediates in the synthesis of polyurethanes, can be controlled by the use of different catalysts and functionalization agents, as well as by varying the polymerization conditions (11 –13). This approach was used by Carothers and is still used by Mitsui Toatsu Chemicals Inc. to manufacture a low to intermediate molecular weight polymer. Addition of acidic catalysts, such as boric or sulfuric acid (14) accelerates the esterification and transesterification processes, but also catalyzes side reactions at temperatures above 1208C. Therefore, polycondensation of aqueous DL -lactic acid never gave Mn’s above 3000 (14, 15), as against Mn’s up to 6500 reported for pure L -lactide. When the precondensates obtained by dehydratization up to 1208C are heated to 1808C in the presence of nonacidic transesterification catalysts, such as PbO, a moderate yield of relatively high-molecular weight PLA may result (16). Yet, even the low molecular weight 330 R. Mehta et al. Figure 3. Preparation of polylactic acid. precondensates may be of interest for the preparation of biodegradable glues or lacquers, because the –OH and – COOH end groups allow cross-linking with suitable inorganic or organic multivalent additives (15). Polycondensation method produces oligomers with average molecular weights several tens of thousands lower than those of PLA synthesized by one-step polycondensation of lactic acid if appropriate azeotropic solvents are employed (17 – 19). This polymer can be used as it is, or can be coupled with isocyanates, epoxides or peroxide to produce polymers having a range of molecular weights. An alternative method, route 2, is discussed below. Synthesis of High Molecular Weight Polylactic Acid by Ring-Opening Polymerization of Lactide Water is removed under mild conditions, without a solvent, to produce a cyclic intermediate dimer, referred to as lactide. This monomer is readily purified by vacuum distillation accomplished by heating, again without the need for solvent. By controlling the purity of the dimer it is possible to produce a wide range of molecular weights. PLA has been produced commercially worldwide since the last decade. The catalyst currently used industrially is stannous octoate (zinc metal has been in use in France). Ringopening polymerization of lactide can be carried out in melt, bulk, or in solution and by cationic, anionic, and coordination-insertion mechanisms depending on the catalyst (20 –22). The choice of initiator system, co-initiator as chain control agent, catalyst concentration, monomer-to-initiator ratio, and polymerization temperature and time significantly affect the polymer properties. These properties, such as the molecular weight, degree of crystallinity and residual monomer content, in turn affect the physical-mechanical properties and range of temperature for use of the polylactide and its copolymers (23 – 29). The role of the racemization and the extent of transesterification in the polymerization and copolymerization process are also decisive for the enantiomeric purity and chain microstructure of the resulting polymer (30 –33). Many current PLA polymerization methods employ stannous octoate as the catalyst. It has been shown to be very effective, causes a low degree of racemization at high temperature (34), has low toxicity, and is accepted by the US Food and Drug Administration. A selective summary of literature on PLA synthesis is given in the Table 4 (35 –51). Other recent studies include dimeric aluminum chloride complexes of N-alkoxyalkyl-b-ketoimines (activated with propylene oxide) (52), alkoxy-amino-bis (phenolate) Table 4 A selective summary of studies on PLA polymerization variables and molecular weight S.No. 1 Polymer D ,L PLA L -PLA 2 3 L -PLA D -L PLA Catalyst Solvent(s) Reaction temp. 8C Reaction time Molecular weight Reference Toluene 70 –100 Up to 100 hrs. Mn . 90,000 Dubois et al. (35) Glycerol Alcohols 130 200 6 hrs. 60– 75 min. DPn ¼ 43-178 Mw , 3,50,000 Han et al. (36) Korhonen et al. (37) Stannous octoate Alcohols, carboxylic acid 130 2 –72 hrs. Mn , 250,000 Zhang et al. (38) Stannous octoate Stannous octoate and triphenylamine Stannous octoate and compounds of titanium and zirconium No solvent No solvent 130 180 –185 72 hrs. 7 min. Toluene 180 –235 15– 180 min. Stannous trifluoromethane sulphonate, Scandium(III) trifluoromethane sulfonate Ethanol 40 –65 50 –100 hrs. DPn ¼ 15– 30 Moller et al. (42) Sn substituted mesoporous silica molecular sieve Mg, Al, Zn, Titanium alkoxides No slovent 130 72 hrs. Mn , 36,000 Fattah et al. (43) Methylene chloride 100 — DPn , 400 Kricheldorf (44) Al Isopropoxide Stannous octoate Stannous octoate L -PLA 4 L -PLA D -L PLA 331 5 6 L -PLA 7 L -PLA L -PLA D -L 8 Mv: ¼ 20,000 –680,000 Hyon et al. (39) Mn ¼ 91,000 Jacobsen et al. (40) Mn ¼ 40,000 – 100,000 Rafier et al. (41) PLA D -PLA L -PLA D -L PLA 9 L -PLA 10 L -PLA (continued ) Table 4 Continued S.No. Polymer 11 L- 12 D -L PLA 13 D -L PLA 14 D -L PLA PLA Catalyst Solvent(s) Reaction temp. 8C Reaction time Molecular weight Reference 332 Yttrium tris(2,6-di-tert butyl phenolate) (in toluene) Butyl lithium, butyl magnesium (in hexane) Zn lactate 2-propanol, butanol, ethanol THF 22 2– 5 min. Mn , 25,000 Stevels et al. (45) — 30 min Mn , 45,000 No solvent 140 96 hrs. Mn ¼ 212,000 Butylmagnesium, Grignard reagent Ethers 0 – 25 4 –8 days Mn , 300,000 Kasperczyk et al. (33) Schwach et al. (46) Kricheldorf et al. (47) Potassium naphthalenide Complexes of iron with acetic, butyric, siobutyric and dichloroacetic acids (Trimethyl triazacyclohexane) praseodymium triflate Lanthanum isopropoxide THF, toluene No solvent 40 170 – 210. 48 –120 hrs. 0.5 –25 hrs. Mn , 16,000 Mw ¼ 150,000 Stere et al.(48) Stolt et al. (49) No solvent 120 – 200 18 hrs. Mv ¼ 10,000 – 20,000 Kohn et al. (50) 21 30 min. Mn ¼ 5300– 21,900 Save et al. (51) 140 – 180 10 –111 hrs. L -PLA 15 16 L -PLA 17 D -L PLA 18 D -L PLA 19 PLA Lead monoxide, lead stearate, (type not basic lead carbonate, antimony specified) trioxide, zinc oxide, zinc borate, cadmium oxide, titanyl stearate, magnesium oxide and calcium formate L -PLA Dichloromethane/ toluene (70/30) No solvent IV (in benzene) ¼ 1.21 Schneider et al. (16) Synthesis of Poly(Lactic Acid) 333 Group 3 metal complexes (53), aluminum complexes bearing tetradentate bis(aminophenoxide) ligands (54), hetero-bimetallic iron(II) alkoxide/aryloxides (55), stannous octoate and diethanolamine (56). b – diiminate ligated magnesium and zinc amides (57), zinc alkoxide complex (58), titanium alkozide (59), iron alkoxide (60), 2,6-dimethyl aryloxide (61), calcium coordination complexes (62), complexes of Cu, Zn, Co and Ni Schiff base derived from salicylidene and L -aspartic acid (63), dizinc-monoalkoxide complex supported by a dinucleating ligand (64), stannous octoate with adducts containing oligomers L -lactide and rac-lactide (65), tertiary amines, phosphines and N-heterocyclic carbenes (66), alkyl aluminum (67) and aluminum – achiral ligand complexes (68). In one of the earlier studies, Baker and Smith (69) documented a procedure of PLA synthesis from racemic materials. In some of the studies, the monomer (lactide) has been used as received (45) and in others it has been used after recrystallizing it from solutions in solvents like chloroform, ethyl acetate, acetone etc. (49). It has been reported that recrystallized L -lactide gives higher intrinsic viscosities than those obtained for the once-recrystallized monomer (44, 47). Also, treatment of the reaction kettle with dichlorodimethyl silane (silanizer) favors a higher molecular weight product. The monomer to initiator ratio has varied from 50 to 50,000 in various studies. The operating conditions have also varied considerably. In some cases stirring of the mixture is employed and in others the reaction kettle is sealed and kept in an oven (38, 46). The reaction environment is either air (47) or an inert gas (70) or vacuum (46). The reaction product is dissolved in an appropriate solvent (CH2Cl2, CHCl3 or acetone) and precipitated into diethyl ether/methanol and then filtered and dried. The polymer identification is done by 1H NMR, 13C NMR and FTIR techniques. Characterization of various PLA by NMR (71) and by IR (72) has been studied. The molecular weights are determined by various ways including measurement of intrinsic viscosity (and calculation of Mn by using Mark-Houwink equation (73)) in chloroform or benzene, gel permeation chromatography, and 13C NMR. The residual solvents are assayed by GC. Single-step Reactive Extrusion In order to make the manufacturing of PLA economically viable, Jacobsen et al. (40) developed a continuous one-stage process using reactive extrusion technology. This technique requires that the bulk polymerization is close to completeness within a very short time (5 –7 min), which is predetermined by the residence time of the extrusion system and that the PLA stability is high enough at the processing temperature. Even though stannous octoate can promote quite fast lactide polymerization, it is also known to have adverse effect on the PLA molecular weight and properties, as a result of backbiting and intermolecular transesterification reactions, not only during the lactide polymerization but also during any further melt processing (74). The authors showed that the addition of an equimolar amount of a Lewis base, particularly triphenylphosphine onto stannous octoate, significantly enhances the lactide polymerization rate in bulk. Also the influence of process parameters on the final polymer properties was studied. The kinetic effect has been accounted for by coordination of the Lewis base onto the metal atom of the initiator making the insertion of the monomer into the metal alkoxide bond of the initiator easier. An important task for developing new catalytic systems is to make the catalyst more compatible for the purpose of biomedical applications. Stannous octaote has been one of the most effective catalysts that give both high yields and high molecular weights. 334 R. Mehta et al. However, like many other catalysts, the cytotoxicity and difficulties in removal of the catalyst from the resulting polymer have limited its utilization in many cases. Additionally, triphenylphosphine is also not likely to be any safer. Continuous Process for Production of PLA from Lactic Acid A continuous process for manufacture of PLA with controlled optical purity (Fig. 4) has been described by Gruber et al. (75 – 80). The process involves forming a low molecular weight condensation product, PLA. This is followed by depolymerizing the polylactic acid Figure 4. Schematic flow chart of the continuous process for the manufacture of PLA from lactic acid (13). Synthesis of Poly(Lactic Acid) 335 in a lactide reactor to form crude lactide, which is purified in a distillation system. A purified lactide is then polymerized to form lactide polymers. The process in detail is as follows. A crude lactic acid feed is provided, which is a solution of about 15% lactic acid and about 85% water, and is available commercially. The feed is concentrated by removing water or any other solvent such as methanol, ethanol etc. or hydrolytic medium, which are used as a carrier for the lactic acid, a partial vacuum may be applied in the evaporator. The lactic acid is concentrated to about 99% and transferred to a prepolymer reactor. The prepolymer reactor is essentially a second evaporator system to further remove water or solvent from the lactic acid. It is known that lactic acid undergoes a condensation reaction to form polylactic acid as water is removed. Thus, polylactic acid up to a molecular weight of about 5000 is prepared in the prepolymer reactor. This is transferred to lactide reactor where an appropriate catalyst and process stablizers are added. The mean residence time in the lactide reactor is kept as low as possible. Thus, falling film and thin-film evaporators are used. The lactide is removed continuously from the reactor as a vapor. The removal of lactide further drives the depolymerization reaction. The lactide vapors are transferred to a distillation unit for purification. The refined lactide is removed from the distillation system and fed to a polymerization reactor for ring-opening polymerization yielding high molecular weight PLA. The crude lactic acid feed to this process may be made up of L -lactic acid or D -lactic acid, or a combination thereof. Racemization or conversion of one optical enantiomer to the other, may occur. Such racemization is driven by such factors as temperature, pressure, and time at a given temperature or pressure, the presence of catalysts or impurities, and relative concentrations of the two enantiomers at any given time. Amorphous films (81 –84) as well as semi-crystalline films (85 – 88) can be made from PLA, in a continuous process. PLA Blends and Composites A review of the PLA blends is given by Kylma (89). There are two main considerations: miscibility or compatability, and biodegradability of the second component. Several blend systems containing PLA have been investigated, such as blends of PLA with poly(1-caprolactone) (90 – 92) poly[(R)-3-hydroxybutyrate] (93 –95), poly[(R)3-hydroxybutyrate-co-(R)-3-hydroxyvalerate] (96), poly(ethylene oxide) (97 – 99) and poly(vinyl acetate) (100). Most of the blends have been found to be immiscible with a phase separated morphology. An interesting phenomena in blends of poly(L -lactide) and poly (D -lactide) is the formation of a stereocomplex. The PLA stereocomplex is found to possess a racemic crystalline structure, where PDLA and PLLA chains are packed side by side with a D monomer unit to L monomer unit in the ratio of 1 : 1. One of the most interesting findings in PLLA/PDLA stereocomplexation studies is that the melting temperature of the stereocomplex is 2308C, approximately 508C above that of the corresponding homopolymer. This enantiomeric polymer blend also exhibits substantially higher tensile properties and better thermal stability and hydrolysis resistance than the polylactides from which the blends are prepared (101, 102). An excellent review of the mechanical properties of biodegradable polymers has been prepared by Daniels and co-workers (Figs. 5 and 6) (103). Totally bioabsorbable composite plates have been made from PGA fibers embedded in a PLA matrix. The reaction time and properties of the PLA can be controlled by making stereo copolymers of D - and L - lactic acid. The number of D -units apparently controls the 336 R. Mehta et al. Figure 5. Representative flexural strengths (MPa) of absorbable polymer composites (103). degradation rate. These composites are bioabsorbable, exhibit good biocompatibility with the tissues in which they are implanted, and have adjustable resorption rates, depending on the relative amounts of L - and D - lactic acid units as well as on the quantities of GA and LA repeating units. This concept of bioabsorption or biodegradability is an important one in many areas of bioimplants (104). Composites of PLA have been made with jute fibers (105) and bioactive glass (106). Nano-composites have been made with organo-modified montmorillonites (107) and silicates (108). Polymerization Mechanism There has been an increasing interest in the development of simple efficient catalytic systems for the ring-opening polymerization of lactide. Some of the polymerization conditions and the molecular weights of the products are also given in Table 4. The mechanism through which the catalyst works has been suggested for some systems. It has been demonstrated that lactone polymerization using aluminium and tin alkoxides proceeds via an insertion mechanism (44, 109, 110). Furthermore, when tin halogenides are used as catalysts, it has been proposed that they are actually converted into tin alkoxides, which are the real active species in the polymerization process (111). Kricheldorf et al. (44) suggested that for various metal alkoxides, the ring opening of Figure 6. Representative flexural moduli (GPa) of abosorbable polymer composites (103). Synthesis of Poly(Lactic Acid) 337 the lactones involves the cleavage of the acyl-oxygen bond and the alkoxide groups of the initiator form alkyl ester end-groups. Dubois et al. (35) suggested that the ring opening polymerization using aluminium isopropoxide proceeds through a ‘coordination – insertion’ mechanism and selective rupture of the acyl-oxygen bond of the monomer, as shown in Fig. 7. Zhang et al. (38) studied the effect of hydroxyl and carboxylic acid substances on lactide polymerization in the presence of stannous octoate. Stannous alkoxide, a reaction product between stannous octoate and alcohol, was proposed as the substance initiating the polymerization through coordinative insertion of lactide. Alcohol could affect the polymerization through reactions leading to initiator formation, chain transfer, and transesterification. Carboxylic acids affect the polymerization though a deactivation reaction. Experiments have shown that alcohol increases PLA production rate while carboxylic acid decreases it. The higher the alcohol concentration, the lower is the polymer molecular weight. However, the final molecular weight of PLA is not sensitive to the carboxylic acid concentration. Stolt and Sodergard (49) reported the ring-opening polymerization of L -lactide usingdifferent organic monocarboxylic iron complexes. It was observed that the acetate anion as well as the iron partly, are chemically attached to the polymer chain, and the proposed polymerization mechanism is an anionic type of coordination insertion as described in Fig. 8. Schwach et al. (112) reexamined the ring-opening polymerization of PLA in the presence of stannous octoate under conditions allowing for the end-group characterization of growing chains by high-resolution 1H-NMR. For low values of monomer to initiator ratios, the DL -lactide ring was opened to yield lactyl octoate-terminated short chains. A cationic-type mechanism involving co-ordination by octanoic acid was proposed to account for experimental findings (Fig. 9). In another work (70), the same group studied the bulk polymerization of PLA using stannous octoate and zinc metal as catalysts. A two-level fractional factorial design was used to assess the influence of selected experimental variables with respect to intermolecular transesterification. Within the range of the selected variables, a hierarchy of average effects was established as: polymerization temperature . monomer-to-initiator ratio . polymerization time . initiator . monomer degassing time. The investigation tool used was 13C NMR. In another study (113), the group reported the polymerization of DL -lactide in the presence Figure 7. The mechanism of PLA polymerization using aluminium isopropoxide as catalyst (35). 338 R. Mehta et al. Figure 8. An anionic type of coordination insertion mechanism for organic monocarboxylic iron complexes as catalysts (49). of zinc metal. The results showed that the polymerization was water sensitive and that only a fraction of zinc was active. A small amount of zinc lactate was present and was proposed to be the actual initiator. Kricheldorf et al. (114) studied the polymerization of racemic and meso DL -lactide at 1208C in xylene solution or in bulk. Lead oxide (PbO), zinc stearate, antimony(III) 2-ethylhexanoate, and bismuth(III) 2-ethylhexanoate were used as initiators. High yields (greater than or equal to 90%) were obtained only with PbO and Bi(III) 2-ethylhexanoate, but the molecular weights were low in all cases. At higher reaction temperatures, the resulting stereosequences showed an increasing tendency toward randomness. In another study (115), the same group tested various acidic compounds as potential initiators of the cationic polymerization of L -lactide. Regardless of the solvent and temperature, only trifluoromethanesulfonic acid and methyl triflate proved to be useful initiators. Stannous(II) triflouromethane sulfonate and scandium(III) trifluoromethane sulfonate have also been studied as catalysts for PLA synthesis (42). It was found that polymers of predictable molecular weights and narrow polydispersities could be obtained. The addition of base either as a solvent or as an additive significantly enhanced the polymerization rate with minimal loss to the polymerization control. Leenslag and Pennings (25) studied the polymerization of L -lactide as a function of polymerization temperature, time and concentration of catalyst (stannous octoate). PLA with the highest value of intrinsic viscosity (Mv ¼ 106) was synthesized at a low catalyst concentration (0.015 wt%) and at the temperature of 1008C. The Mw/Mn ratios of as-polymerized PLA samples ranged from 2 to 3. The experimental results suggested a nonionic insertion polymerization mechanism. In contrast to this study, using the same catalyst, Hyon et al. (39) obtained PLA with the maximum molecular weight at a Synthesis of Poly(Lactic Acid) 339 Figure 9. Cationic octanoic acid co-initiated mechanism of lactide polymerization in presence of stannous octoate (112). catalyst concentration of 0.05% at 1308C. In this study, the decrease in Mv at prolonged polymerization and higher polymerization temperature was attributed to thermal depolymerization of the resultant polylactides. In contrast to this, the drop in Mn in the polymerization using aluminium isopropoxide (35) at higher temperatures and higher monomer-to-initiator ratio was attributed to intra- and inter-molecular transesterification reactions. Nijenhuis et al. (116) studied the kinetics and mechanism of L -lactide bulk polymerization using stannous octoate and zinc bis(2,2-dimethyl-3,5-heptanedionate-O,O0 ). Up to 80% conversion, the rate of polymerization using a tin compound was higher than that with zinc-containing catalyst, while at conversions beyond 80%, the latter catalyst gave the higher rate of polymerization. Crystallization of the newly formed polymer has an accelerating effect on the polymerization. The differences in the rate of polymerizations at high conversion for the two catalysts are suggested to be caused by a difference in crystallinity of the newly formed polymer. It is further suggested that contaminants in the catalyst and the monomer are the true initiators. Initiation as well as polymerization 340 R. Mehta et al. proceeds through a Lewis acid catalyzed transesterification reaction between an activated lactone and a hydroxyl group. Reaction Kinetics Considerable work has been done on the study of reaction kinetics. The nature of the chain-growth process in ring-opening polymerization bears a superficial resemblance to chain polymerization. Only monomer adds to the growing chain in the propagation step. Species larger than monomer do not react with the growing chains. However, ring-opening polymerizations can have the characteristics of either chain or step polymerization or both (117). Initiation prepares an ionic reactive centre, which adds many monomer units in a chain reaction or coordination reaction (propagation) and grows to a large size. The chain produced may be ‘living’ or terminated. Initiation results in opening of the ring to form secondary initiator species M , which may be either an ion or neutral molecule depending on the initiator. This can be generalized as R----Z þ C ! M ð1Þ where Z is the functional group in the monomer and C is the ionic or molecular initiator. The initiator species grow by successive ring-opening additions of many monomer molecules M þ nRZ ! M---ðRZÞn ð2Þ Dubois et al. (35) found that the reaction was of first order with respect to monomer or initiator (aluminum isopropoxide) and was given by the following equation: d½M ¼ k½M½I dt ð3Þ where [M] and [I] are monomer and initiator concentrations. They calculated the value of rate constant, k, as 0.6 L mol21 min21. Schwach et al. (46) using zinc lactate as catalyst found k to be equal to 0.045 L/mol . hr. They also found the rate constant to be 8 times higher for stannous octoate compared to zinc lactate (118). However, this rate constant, k, is only an apparent rate constant since it does not represent the actual reactions occurring in the reaction vessel. The difficulties in experimental determination of the rate constants are discussed by Odian (117), and are mentioned herein. Under several assumptions (including the assumption of steady state i.e. the rate of initiation is equal to the rate of termination) the ratio of rate constants (propagation rate constant/rate constant for termination by transfer to monomer) can be obtained if the variation of number average degree of polymerization with monomer concentration is known. The determination of individual rate constants requires the determination of kp, a difficult task and one that has not been performed properly. This requires the critical evaluation of the concentration of the propagating species, which should not be taken as equal to the concentration of the initiator without any experimental verification (such an assumption holds only if the rate of propagation is much less than the rate of initiation). There are two general methods for the experimental evaluation of this concentration, neither approach being experimentally simple or unambiguous (117). One method involves quickly stopping the polymerization process by adding a highly effective terminating agent and Synthesis of Poly(Lactic Acid) 341 analyzing the end-groups (119). The second method involves UV spectroscopic analysis of the propagating species during polymerization (120). Evaluation of rate constants by modeling and simulation in conjunction with the experimental results offers several advantages: initiation, propagation and termination rate constants can be evaluated; termination mechanism can be ascertained and lastly chain dependent rate constants can be evaluated. The authors have made some effort in this direction. For reference an example is given here for the evaluation of the rate constants for the ring-opening polymerization of PLA using iron isobutyrate as catalyst. The kinetic scheme can be represented as: Initiation: ki I þ M ! P1 ð4Þ Propagation: kp Pj þ M ! P jþ1 ð5Þ Termination by transfer to monomer: kt;M Pj þ M ! Mj þ P1 ð6Þ where [Pj] denotes the concentration of polymers of chain length j, [M] denotes concentration of the monomer. In equation (6), it is assumed that the charged ring spontaneously forms P1. Here Mj is the deactivated polymer of j repeat units, which will not participate in any reaction. The number average molecular weight, Mn and weight average molecular weight, Mw are calculated as: n P Mn ¼ m j¼1 n P jð½Pj þ ½Mj Þ ð7Þ ð½Pj þ ½Mj Þ j¼1 n P Mw ¼ m j¼1 n P j2 ð½Pj þ ½Mj Þ ð8Þ jð½Pj þ ½Mj Þ j¼1 where m is the molecular weight of the repeating unit. Mass balance equations for a batch reactor may be written for this kinetic scheme as follows: n n X X d½M ¼ ½Mfki ½I þ k pj ½Pj þ kt;Mj ½Pj g dt j¼1 j¼1 d½I ¼ ki ½I½M dt n X d½P1 ¼ ki ½I½M k p1 ½P1 ½M þ kt;Mj ½Pj ½M dt j¼2 ð9Þ ð10Þ ð11Þ 342 R. Mehta et al. d½Pj ¼ ½Mfk pð j1Þ ½P j1 k pj ½Pj kt;Mj ½Pj g; dt d½Mj ¼ kt;Mj ½Pj ½M; j 1 dt j.1 ð12Þ ð13Þ With initial conditions, at t ¼ 0 ½M j ¼ 0 ½M ¼ ½M 0 ½I ¼ ½I 0 and ½Pj ¼ 0; j1 ð14Þ ð15Þ ð16Þ where [I0] and [M0] are the initial molar concentrations of the initiator and the monomer, respectively. The square brackets represent molar concentrations and subscripts of rate constants show chain length dependent values. It was subsequently assumed that rate constants are chain length independent. Differential equations were solved using Euler’s method on a PC using Pascal. Euler’s method was used in place of more sophisticated ODEs methods because it was found to be sufficiently accurate for our purpose. This was confirmed by obtaining the limiting case of Poisson distribution in a simulation where the termination constant was taken to be zero and a relatively large initiation rate constant was considered. A large value of n (n ¼ 5000) was used for all simulations. The Mn and Mw were calculated as a function of polymerization time, for different monomer/initiator ratio, and were matched with the reported results (49) as shown in Fig. 10. Simulations were run to match the numerical curves with the reported data and values of parameters were determined by trial and error approach. The values of polydispersity obtained from modeling are slightly lower than Figure 10. Comparison of experimental (49) and model predicted results for the polymerization of PLLA catalyzed with Iron Isobutyrate, at 1908C. The weight-average molecular weight vs. polymerization time, have been plotted. The experimental polydispersity is noted in parenthesis and the modeled polydispersity is shown below it. The solid lines are the solutions obtained from the model. Synthesis of Poly(Lactic Acid) 343 the experimental values. This could be due to the transesterification reaction. The values of the rate constants determined are: kp ¼ 31.5 L/mol . min, ki ¼ 0.02 L/mol . min, and kt,M ¼ 0.025 L/mol.min. It should be noted that since the synthesis of PLA in 1932, this is the first attempt to report individual polymerization rate constants (kp, ki and kt,M). It should be mentioned that there would be some inaccuracy involved in the results stemming from the poor reproducibility, in general, of the ionic polymerization data. Thermodynamics: Equilibrium Monomer Conversion Lactides are six-membered cyclics, and the reversibility of their polymerization could be expected. Polymerization of lactides never reaches 100% conversion, and yields .95% require polymerization temperature 1808C. Very little experimental data is available on the thermodynamics of the propagation-depropagation steps. Thermodyanamics of L -lactide polymerization in 1,4-dioxane solvent was studied by Duda and Penczek (121). The equilibrium concentration of L -lactide, as measured by gel permeation chromatography, decreased from 0.15 mol . L21 at 406 K to 0.06 mol/L at 353 K. The standard thermodynamic parameters, determined on the basis of the temperature dependence of the L -lactide $ poly(L -lactide) equilibrium position were as follows: enthalpy ¼ 222.9 kJ/mol, entropy ¼ 241.1 J/mol.K (at 1 mol/L). Negative values of enthalpy and entropy lead to the existence of ceiling temperature, Tc ¼ 914 K (value computed for the bulk polymerization). The relatively high value of polymerization enthalpy compared to that of other six-member monomers was attributed to the bond oppositions and angle distortions in the skew-boat conformation of the L -lactide molecule. Conclusions It has been known for over half a century that high molecular weight PLA can be produced by the ring-opening polymerization of lactide. The number of catalysts, which have been reported to initiate this polymerization, is staggering. However, there is still a need for a safer, faster and a more stable catalyst. Though a single-step extrusion process has been developed, there are questions about the safety of the catalysts which are left in the final polymer, subsequently used in human body applications. The information about the modeling of ring-opening polymerization is lacking. Regarding the future prospects, it is expected that PLA will in a few years achieve the status of a commodity polymer. References 1. Fruzza, E.J. and Schmitt, E.E. (1971) A new absorbable suture. J. Biomed. Mat. Res., 1: 43 – 58. 2. Gilding, D.K. and Reed, A.M. (1981) Biodegradable polymers for use in surgery: PGA/PLA homo- and copolymers. Polymer, 22: 494– 498. 3. Ratner, B.D., Hoffman, A.S., Schoen, F.J., and Lemons, J.E. (1996) Biomaterials Science: An Introduction to Materials in Medicine. Society of Biomaterials, Academic Press: San Diego, Ch. 2, 37– 130. 4. Williams, D.F. (1987) Definitions in Biomaterials. Proceedings of a Consensus Conference of the European Society for Biomaterials. Elsevier: New York. 5. Vert, M., Li, S.M., Spenlehauer, G., and Guerin, P. (1992) Bioresorbability and biocompatibility of aliphatic polyesters. J. Mater. Sci: Mater. Med., 3: 432– 446. 6. Wandsworth, L. (1993) Melt processing of PLA resin into nonwovens, 3rd Annual TANDEC Conference, Knoxville. 344 R. Mehta et al. 7. www.plasticstechnology.com/articles/200203fa2.html (accessed August 2004). 8. Engleberg, I. and Kohn, J. (1991) Physicomechanical properties of degradable polymers used in medical applications. A comparitive study. Biomaterials, 12: 292– 304. 9. Thakur, K.A.M., Kean, R.T., Zupfer, J.M., Buehler, N.U., Doscotch, M.A., and Munson, E.J. (1996) Solid state 13C CP-MAS NMR studies of the crystallinity and morphology of poly(L -lactide). Macromolecules, 29: 8844– 8851. 10. Fambri, L., Pegoretti, A., Fenner, R., Incardona, S.D., and Migliaresi, C. (1997) Biodegradable fibers of poly(L -lactic acid) produced by melt spinning. Polymer, 38: 79 – 85. 11. Hiltunen, K., Seppälä, J.V., and Härkönen, M. (1997) The effect of catalyst and polymerization conditions in the preparation of low molecular weight lactic acid polymers. Macromolecules, 30: 373– 379. 12. Hiltunen, K. and Seppälä, J.V. (1998) The use of different diols in the synthesis of low-molecular weight lactic-acid-based telechelic prepolymers. J. Appl. Polym. Sci., 67: 1017 –1023. 13. Gruber, P.R., Hall, E.S., Kolstad, J.J., Iwen, M.L., Benson, R.D., and Borchordt, R.L. (1993) Continuous process for manufacture of a purified lactide. US Patent 5,274,073. 14. Filachone, E.M. and Fisher, C.H. (1944) Lactic acid condensation polymers. Ind. Eng. Chem, 36: 223– 228. 15. Watson, P.D. (1948) Lactic acid polymers as constituents of synthetic resins and coatings. Ind. Eng. Chem., 40: 1393– 1397. 16. Schneider, A.K. and Wilmington, D. (1955) Properties of high melting lactide. U.S. Patent 2,703,316, March 1. 17. Lunt, J. (1998) Large-scale production, properties and commercial applications of polylactic acid polymers. Polymer Degradation and Stability, 59: 145– 152. 18. http://www.cargilldow.com (accessed May 2004). 19. Hyon, S., Jamshidi, K., and Ikada, Y. (1997) Synthesis of polylactides with different molecular weights. Biomaterials, 18: 1503– 1508. 20. Mecerreyes, D., Jérôme, R., and Dubois, P. (1999) Novel macromolecular architectures based on aliphatic polyesters: Relevance of the “coordination-insertion” ring-opening polymerization. Adv. Polym. Sci., 147: 1 – 59. 21. Nieuwenhuis, J. (1992) Synthesis of polylactides, polyglycolides and their copolymers. Clin. Mater., 10: 59 – 67. 22. Löfgren, A., Albertsson, A.-C., Dubois, P., and Jérome, R. (1995) Recent advances in ringopening polymerization of lactones and related compounds. J. Macromol. Sci.-Rev. Macromol. Chem. Phys., C35: 379– 418. 23. Vert, M., Schwarch, G., and Coudane, J. (1995) Present and future of PLA polymers. J.M.S.-Pure Appl. Chem., A32: 787–796. 24. Kim, S.H., Han, Y.-K., Ahn, K.-D., Kim, Y.H., and Chang, T. (1993) Preparation of star-shaped polylactide with pentaerythritol and stannous octoate. Macromol. Chem., 194: 3229 –3236. 25. Leenslag, J.W. and Pennings, A.J. (1987) Synthesis of high-molecular-weight poly(L -lactide) initiated with tin 2-ethylhexanoate. Macromol. Chem., 188: 1809–1814. 26. Vion, J.-M., Jérôme, R., Teyssié, P., Aubin, M., and Prud’homme, R.E. (1986) Synthesis, characterization, and miscibility of caprolactone random copolymers. Macromolecules, 19: 1828– 1838. 27. Grijpma, D.W. and Pennings, A.J. (1991) Polymerization temperature effects on the properties of L -lactide and g-caprolactone copolymers. Polym. Bull., 25: 335– 341. 28. Prego, G., Cella, G.D., and Bastioli, C. (1996) Effect of molecular weight and crystallinity on poly(lactic acid) mechanical properties. J. Appl. Polym. Sci., 59: 37 – 43. 29. Duda, A., Penczek, S., and Kowalski, A. (2000) Libiszowski polymerization of e-caprolactone and L , L -dilactide initiated with stannous octoate and stannous butoxide—a comparison. Macromol. Symp., 153: 41 – 53. 30. Chabot, F., Vert, M., Chapelle, S., and Granger, P. (1983) Configurational structures of lactic acid stereocopolymers as determined by 13C– 1H. Polymer, 24: 53 – 59. Synthesis of Poly(Lactic Acid) 345 31. Bero, M., Kasperczyk, J., and Jedlinski, Z.J. (1990) Coordination polymerization of lactides, 1. Structure determination of obtained polymers. Macromol. Chem., 191: 2287– 2296. 32. Kricheldorf, H.R. and Kreiser, I. (1987) Polylactones. 13. Transesterification of poly(L -lactide) with poly(glycolide), poly(b-propiolactone), and poly(g-caprolactone). J. Macromol. Sci. Chem., A24: 1345– 1356. 33. Kasperczyk, J. and Bero, M. (2000) Stereoselective polymerization of racemic DL -lactide in the presence of butyllithium and butylmagnesium. Structural investigations of the polymers. Polymer, 41: 391– 395. 34. Kricheldorf, H.R. and Serra, A. (1985) Polylactones. 6: Influence of various metal salts on the optical purity of poly(L -lactide). Polym. Bull., 14: 497– 502. 35. Dubois, Ph., Jacobs, C., Jerome, R., and Teyssie, Ph. (1991) Macromolecular engineering of polylactones and polylactides. Mechanism and kinetics of lactide homopolymerization by aluminum isopropoxide. Macromolecules, 24: 2266– 2270. 36. Han, D.K. and Hubbell, J.A. (1996) Lactide-based poly(ethylene glycol) polymer networks for scaffolds in tissue engineering. Macromolecules, 29: 5233– 5235. 37. Korhonen, H., Helminen, A., and Seppala, J.V. (2001) Synthesis of polylactide in the presence of co-initiators with different number of hydroxyl groups. Polymer, 42: 7541– 7549. 38. Zhang, X., MacDonald, D.A., Goosen, M.F., and McAuley, K.B. (1994) Mechanism of lactide polymerization in the presence of stannous octoate: The effect of hydroxyl and carboxylic acid substances. J. Polym. Sci. Part A: Poly. Chem., 32: 2965– 2970. 39. Hyon, S.H., Jamshidi, K., and Ikada, Y. (1997) Synthesis of polylactides with different molecular weights. Biomaterials, 18: 1503 –1508. 40. Jacobsen, S., Fritz, H.G., Degee, P., Dubois, P., and Jerome, R. (2000) New developments on the ring-opening polymerization of polylactide. Industrial Crops and Products, 11 (2 – 3): 265– 275. 41. Rafier, G., Lang, J., Jobmann, M. and Bechthhold, I. (2003) Process for manufacturing homoand copolyesters of lactic acid. U.S. Patent 6, 657,042, Dec. 2. 42. Moller, M., Nederberg, F., Lim, L.S., Kange, R., Hawker, C.J., Hedrick, J.L., Gu, Y., Shah, R., and Abbott, L. (2001) Stannous(II) trifloromethane sulfonate: a versatile catalyst for the controlled ring-opening polymerization of lactides: formation of stereo-regular surfaces from polylactide brushes. Journal of Polymer Sciene: Part A: Polymer Chemistry, 39: 3529– 3538. 43. AbdelFattah, T.M. and Pinnavata, T.J. (1996) Substituted mesoporous silica molecular sieve (Si-HMS): Synthesis and properties as a heterogeneous catalyst for lactide ring-opening polymerization. Chem. Commun., 5: 665– 666. 44. Kricheldorf, H.R., Berl, M., and Scharnagi, N. (1998) Polylactones: 9 Polymerization mechanism of metal alkoxide-initiated polymerizations of lacide and various lactones. Macromolecules, 21: 286– 293. 45. Stevels, W.M., Ankone, M.J.K., Dijkstra, P.J., and Feijen, J. (1995) Well defined block copolymers of 1-caprolactone and L -lactide using Y5(m-O)(OiPr)13 as an initiator. Macromol. Chem. Phy., 196: 1153– 1161. 46. Schwach, G., Coudane, J., Engel, R., and Vert, M. (1996) Zinc lactate as initiator of DL -lactide ring-opening polymerization and comparison with stannous octoate. Polym. Bull., 37: 771– 776. 47. Kricheldorf, H.R. and Lee, S.R. (1995) Polylactones: 32 High-molecular weight polylactides by ring-opening polymerization with dibuthylmagnesium or butylmagnesium chloride. Polymer, 36: 2995– 3003. 48. Stere, C., Lovu, M., Boborodea, A., Vasilescu, D.S., and Fazakas-Anca, L.S. (1998) Anionic and ionic coordination polymerization of L -lactide. Polymer Adv. Techno., 9: 322– 325. 49. Stolt, M. and Sodergard, A. (1999) Use of monocarboxylic iron derivatives in the ring-opening polymerization of L -lacide. Macromolecules, 32: 6412– 6417. 50. Kohn, R.D., Pan, Z., Sun, J., and Liang, C. (2003) Ring-opening polymerization of D ,L -lactide with bis(trimethyl triazacyclohexane) praseodymium triflate. Catalysis Communication, 4 (1): 33 – 37. 346 R. Mehta et al. 51. Save, M., Schappacher, M., and Soum, A. (2002) Controlled ring-opening polymerization of lactones and lactide initiated by lanthanum isopropoxide. General aspects and kinetics. Macromol. Chem. Phys., 203 (5/6): 889– 899. 52. Doherty, S., Errington, R., Housley, N., and Clegg, W. (2004) Dimeric aluminum chloride complexes of n-alkoxyalkyl-b-ketoimines: Activation with propylene oxide to form efficient lactide polymerization catalysts. Organometallics, 23 (10): 2382– 2388. 53. Cai, C.X., Amgoune, A., Lehmann, C.W., and Carpenter, J.F. (2004) Stereoselective ringopening polymerization of racemic lactide using alkozy-amino-bis(phenolate) group 3 metal complexes. Chemical Communications, 3: 330– 331. 54. Hormnirm, P., Marshall, E.L., Gibson, V.C., White, A.J., and Williams, D.J. (2004) Remarkable stereocontrol in the polymerization of racemic lactide using aluminum initiators supported by tetradentate aminophenoxide ligands. J. Am. Chem. Soc., 126 (9): 2688– 2689. 55. McGuinness, D.S., Marshall, E.L., Gibson, V.C., and Steed, J.W. (2003) Anionic iron(II) alkoxides as initiators for the controlled ring-opening polymerization of lactide. Journal of Polymer Science, Part A: Polymer Chemistry, 41 (23): 3798– 3803. 56. Li, Y.X., Wang, X., Gao, J.W., Liao, K.R., and Quan, D.P. (2003) Synthesis and characterization of polylactide using diethanolamine as co-initiators. Zhongsahn Daxue Xuebac, Ziran Kexueban (Chinese), 42 (2): 42 – 45. 57. Chrisholm, M.H. and Phomphrai, K. (2003) Conformational effects in b-diiminate ligated magnesium and zinc amides. Solution dynamics and lactide polymerization. Inorganica Chimica Acta, 350: 121– 125. 58. Williams, C.K., Breyfogie, L.E., Choi, S.K., Nam, W., and Young, V.G. (2003) A highly active zinc catalyst for the controlled polymerization of lactide. J. Am. Chem. Soc., 125 (37): 11350– 11359. 59. Kim, Y., Jnaneshwara, G.K., and Verkada, J.G. (2003) Titanium alkoxides as initiators for the controlled polymerization of lactide. Inorganic Chemistry, 42 (5): 1437– 1447. 60. Gibson, V.C., Marshall, E.L., Navarro, L., White, A.J.P., and Williams, D.J. (2002) A well defined iron(II) alkoxide initiator for the controlled polymerization of lactide. Journal of the Chemical Society, Dalton Transactions, 23: 4321–4322. 61. Zhang, L., Shen, Z., Yu, C., and Fan, L. (2004) Ring-opening polymerization of D ,L -lactide by rare earth 2,6-dimethylarylxide. Polymer International, 53: 1013– 1016. 62. Chrisholm, M.H., Calluci, J., and Pompphrai, K. (2003) Lactide polymerization by welldefined calcium coordination complexes: Comparisons with related magnesium and zinc chemisty. Chemical Communications, 1: 48 – 49. 63. Sun, J., Shi, W., Chen, D., and Liang, C. (2002) The ring-opening polymerization of D ,L - lactide catalyzed by new complexes of Cu, Zn, Co, and Ni Schiff base derived from salicylidene and L -aspartic acid. Journal of Applied Polymer Science, 86 (13): 3312– 3315. 64. Williams, C.K., Brooks, N.R., Hillmyer, M.A., and Tolman, W.B. (2002) Metalloenxyme inspired dizinc catalyst for the polymerization of lactide. Chemical Communications, 18: 2132– 2133. 65. Storey, R.F., Mullen, B.D., Desai, G.S., Sherman, J.W., and Tang, C.N. (2002) Soluble tin(II) macroinitiator adducts for the controlled ring-opening polymerization of lactones and cyclic carbonates. Journal of Polymer Science, Part A: Polymer Chemistry, 40 (20): 3434– 3442. 66. Connor, E.F., Nyce, G., Moeck, A., Myers, M., Nederberg, F., and Hedrick, J.L. (2002) Ringopening polymerization of lactides using nucleophilic organic catalysts. Polymer Preprints, 43 (1): 647. 67. Chang, N.C. and Sun, W.H. (2002) Method of polymerization of lactide and polylactide homopolymers thereof. US Patent 6,376,643, April 23. 68. Nomura, N., Ishi, R., Akakura, M., and Aoi, K. (2002) Stereoselective ring-opening polymerization of racemicic lactide using aluminum-achiral ligand complexes: Exploration of a chain-end control mechanism. J. Am. Chem. Soc., 124: 5938– 5939. 69. Baker, G.L. and Smith, M.R. (2002) Process for the preparation of polymers of dimeric cyclic esters. U.S. Patent 6,469,133, Oct. 22. Synthesis of Poly(Lactic Acid) 347 70. Schwach, G., Coudane, J., Engel, R., and Vert, M. (1994) Stannous octoate- versus zinc-iniated polymerization of racemic lactide. Polym. Bull., 32: 617– 623. 71. Kasperczy, J.E. (1999) HETCOR NMR study of poly(rac-lactide) and poly(meso-lactide). Polymer, 41: 5455– 5458. 72. Kisher, G., Cassanas, G., and Vert, M. (1998) Effect of morphology, conformation and configuration on the IR and Raman spectra of various polylactic acids. Polymer, 39: 267– 273. 73. Schindler,; Harper, D. (1979) Polylactide. II. Viscosity – molecular weight relationships and unperturbed chain dimensions. J. Polym. Sci. Polym. Chem. Edn, 17: 2593– 2599. 74. Gogolewshi, S., Janovoic, M., Perren, S.M., Dhillon, J.G., and Hughes, M.K. (1993) The effect of melt-processing on the degradation of selected polyhydroxyacids: polylactides, polyhydroxybutyrate, and polyhydroxybutyrate-co-valerates. Poly. Degrad. Stab., 40: 313. 75. Gruber, P.R. et al. (2001) Continuous process for the manufacture of lactide and lactide polymers. US Patent 6,326,458, Dec. 4. 76. Gruber, P.R. et al. (1992) Continuous process for manufacture of lactide polymers with controlled optical purity. US Patent 5,142,023, Aug. 25. 77. Gruber, P.R. et al. (1993) Continuous process for manufacture of lactide polymers with controlled optical purity. US Patent 5,258,488, Nov. 2. 78. Gruber, P.R. et al. (1994) Melt-stable lactide polymer composition and process for manufacture thereof. US Patent 5,338,822, Aug. 16. 79. Gruber, P.R. et al. (1999) Continuous process for manufacture of lactide polymers with controlled optical purity. US Patent 6,005,067, Dec. 21. 80. Gruber, P.R. et al. (2001) Continuous process for manufacture of lactide polymers with controlled optical purity. US Patent 6,277,951, Aug. 21. 81. Gruber, P.R., Hall, E.S., Kolstad, J.J., Ryan, C.M. and Conn, R.S. (1996) Melt-stable amorphous lactide polymer film and process for manufacture thereof. U.S. Patent 5585191, Dec. 17. 82. Gruber, P.R., Hall, E.S., Kolstad, J.J., Ryan, C.M., and Conn, R.S. (1998) Melt-stable amorphous lactide polymer film and process for manufacture thereof. US Patent 5,798,436, Aug. 25. 83. Gruber, P.R., Hall, E.S., Kolstad, J.J., Ryan, C.M., and Conn, R.S. (1999) Melt-stable amorphous lactide polymer film and process for manufacture thereof. US Patent 6,005.068, Dec. 21. 84. Gruber, P.R., Hall, E.S., Kolstad, J.J., Ryan, C.M., and Conn, R.S. (2001) Melt-stable amorphous lactide polymer film and process for manufacture thereof. US Patent 6,207,792, March 27. 85. Gruber, P.R., Kolstad, J.J., and Ryan, C.M. (1996) Melt-stable semi-crystalline lactide polymer film and process for manufacture thereof. US Patent 5536807, July 16. 86. Gruber, P.R., Kolstad, J.J., and Ryan, C.M. (1998) Melt-stable semi-crystalline lactide polymer film and process for manufacture thereof. US Patent 5,773,562, June 30. 87. Gruber, P.R., Kolstad, J.J., and Ryan, C.M. (2000) Melt-stable semi-crystalline lactide polymer film and process for manufacture thereof. US Patent 6,093,791, July 25. 88. Gruber, P.R., Kolstad, J.J., and Ryan, C.M. (2000) Melt-stable semi-crystalline lactide polymer film and process for manufacture thereof. US Patent 6, 121,410, Sept. 19. 89. Kylma, J. (2001) Lactic acid based poly (ester urethane)—Modification via copolymerization, chain linking and blending. Ph. D. thesis, Helsinki University of Technology. 90. Hiljanen-Vainio, M., Varpomaa, P., Seppälä, J., and Törmälä, P. (1996) Modification of poly(L -lactides) by blending: mechanical and hydrolytical behavior. Macromol. Chem. Phys., 197: 1503– 1523. 91. Tsuji, H. and Ikada, Y. (1996) Blends of aliphatic polyesters. 1. Physical properties and morphologies of solution-cast blends from poly(D,L -lactide) and poly(1-caprolactone). J. Appl Polym. Sci., 60: 2367– 2375. 92. Meredith, J.C. and Amis, E.J. (2000) LCST phase separation in biodegradable polymer blends: poly(D ,L -lactide) and poly(1-caprolactone). Macromol. Chem. Phys., 201: 733– 739. 348 R. Mehta et al. 93. Blümm, E. and Owen, A.J. (1995) Miscibility, crystallization and melting of poly(3-hydroxybutyrate)/poly(L -lactide) blends. Polymer, 36: 4077– 4081. 94. Koyama, Y. and Doi, Y. (1997) Miscibility of binary blends of poly[(R)-3-hydroxybutyric acid] and poly[(S)-lactic acid]. Polymer, 38: 1589– 1593. 95. Ohkoshi, I., Abe, H., and Doi, Y. (2000) Miscibility and solid-state structures for blends of poly[(S)-lactide] with atactic poly[(R,S)-3-hydroxybutyrate]. Polymer, 41: 5985– 5992. 96. Iannace, S., Ambrosio, L., Huang, S.J., and Nicolais, L. (1994) Poly(3-hydroxybutyrate)co-(3-hydroxyvalerate)/poly-L -lactide blends: Thermal and mechanical properties. J. Appl. Polym. Sci., 54: 1525– 1536. 97. Nakafuku, C. and Sakoda, M. (1993) Melting and crystallization of poly (L -lactic acid) and poly(ethylene oxide) binary mixture. Polym. J., 25: 909– 915. 98. Sheth, M., Kumar, R.A., Davé, V., Gross, R.A., and McCarthy, S.P. (1997) Biodegradable polymer blends of poly(lactic acid) and poly(ethylene glycol). J. Appl. Polym. Sci., 66: 1495– 1505. 99. Nijenhuis, A.J., Colstee, E., Grijpma, D.W., and Pennings, A.J. (1996) High molecular weight poly(L-lactide) and poly(ethylene oxide) blends: Thermal characterization and physical properties. Polymer, 37: 5849 –5857. 100. Gajria, A.M., Davé, V., Gross, R.A., and McCarthy, S.P. (1996) Miscibility and biodegradability of blends of poly(lactic acid) and poly(vinyl acetate). Polymer, 37: 437– 444. 101. Brochu, S., Prud’homme, R.E., Barakat, I., and Jérôme, R. (1995) Stereocomplexation and morphology of polylactides. Macromolecules, 28: 5230–5239. 102. Ikada, Y., Jamshidi, K., Tsuji, H., and Hyon, S.-H. (1987) Stereocomplex formation between enantiomeric poly(lactides). Macromolecules, 20: 904– 906. 103. Daniel, A.U., Chang, M.K.O., and Andriano, K.P. (1990) Mechanical properties of biodegradable polymers and composites proposed for internal fixation of bone. J. Appl. Biomat., 1 (1): 57 – 78. 104. Boretos, J.W. and Eden, M. eds. (1984) Contemporary Biomaterials: Material and Host Response, Clinical Applications, New Technology and Legal Aspects. Noyes Med. Publ.: Park Ridge, NJ. 105. Ouchi, T., Kontani, T., and Ohya, Y. (2003) Modification of polylactide upon physical properties by solution-cast blends from physical and polylactide-grafted dextran. Polymer, 44 (14): 3927– 3933. 106. Roether, J.A., Gough, J.E., and Jerome, R. (2002) Novel bioresorbable and bioactive glass and polylactide for bone tissue engineering. Journal of Materials Science: Materials in Medicine, 13 (12): 1207– 1214. 107. Paul, M.A., Alexandre, M., Degee, P., and Dubois, P. (2003) New nanocomposite materials based on plasticized poly(L -lactide) and organo-modified montmorillonites: Thermal and morphological study. Polymer, 44 (2): 443– 450. 108. Sinha, S.R., Yamada, K., Okamoto, M., and Ueda, K. (2003) New polylactide-layered silicate nanocomposites. 2. Concurrent improvements of material properties, biodegradability and melt rheology. Polymer, 44 (3): 857 –866. 109. Barakat, I., Dubois, P., Jerome, R., and Teyssie, P. (1993) Macromolecular engineering of polylactones and polylactides. X. Selective end-functionalization of poly(D ,L )-lactide. J. Polym. Sci. Polym. Chem., 31: 505– 514. 110. Mukaiyama, T., Ichikawa, J., and Asami, M. (1983) A facile synthesis of carboxylic esters and carboxamides by the use of 1,10 -dimethyl-stannocene as a condensing reagent. Chem. Lett., 5: 683– 686. 111. Kricheldorf, H.R. and Sumbel, M. (1989) Polylactones—18. polymerization of L,L -lactide with Sn(II) and Sn(IV) halogenides. Eur. Polym. J., 25: 585– 591. 112. Schwach, G., Coudane, J., Engel, R., and Vert, M. (1997) More about the polymerization of lactides in the presence of stannous octoate. Journal of Polymer Science Part A: Polymer Chemistry, 35 (16): 3431– 3440. Synthesis of Poly(Lactic Acid) 349 113. Schwach, G., Coudane, J., Engel, R., and Vert, M. (1998) Ring-opening polymerization of D ,L -lactide in the presence of zinc metal and zinc lactate. Polymer International, 46 (3): 177– 182. 114. Kricheldorf, H.R. and Boettcher, C. (1993) Polylactones. XXV, Polymerization of racemic and meso-D ,L -lactide and Zn, Pb, and Bi salts-stereochemical aspects. Journal of Macromolecular Science-Pure and Applied Chemistry, A30 (6 – 7): 441– 448. 115. Kricheldorf, H.R. and Dunsing, R. (1985) Polylactones, 8. Mechanism of cationic polymerizations of L ,L -dilactide. Die Makromolekulare Chemie, 187 (7): 1611– 1625. 116. Nijenhuis, A.J., Grijpma, D.W., and Pennings, A.J. (1992) Lewis acid catalyzed polymerization of L -lactide- kinetics and mechanism of the bulk polymerization. Macromolecules, 25: 6419– 6424. 117. Odian, G. (1991) Principles of Polymerization. Wiley-Interscience: New York. 118. Schwach, G.G. Ph.D Thesis, University Montpellier: France, Feb. 22. 119. Higashimura, T., Kusano, H., Masuda, T., and Okamura, S. (1971) Rate constant of propagation in the cationic polymerization of styrene catalyzed by BF3O(C2 H5)2. J. Polym. Sci. Polym. Lett. Ed., 9: 463– 466. 120. Sawamoto, M. and Higashimura, T. (1978) Stopped-flow study of the cationic polymerization of styrene derivatives. 1. Direct observation of the propagating species in the polymerization of p-methoxystyrene in 1,2-dichloroethane. Macromolecules, 11: 328– 332. 121. Duda, A. and Penczek, S. (1990) Thermodynamics of L -lactide polymerization. Equilibrium monomer concentration. Macromolecules, 23: 1636– 1639.